Polydisperse methyl β-cyclodextrin–epichlorohydrin ... · PDF file NMR...
Embed Size (px)
Transcript of Polydisperse methyl β-cyclodextrin–epichlorohydrin ... · PDF file NMR...
Polydisperse methyl β-cyclodextrin–epichlorohydrin polymers: variable contact time 13C CP-MAS solid-state NMR characterization Isabelle Mallard1, Davy Baudelet1,2,3, Franca Castiglione4, Monica Ferro4, Walter Panzeri5, Enzio Ragg6 and Andrea Mele*4,5,§
Full Research Paper Open Access Address: 1ULCO, UCEIV, F-59140 Dunkerque, France, 2UCLille, EA GRIIOT (4481), Laboratoire de Pharmacochimie, HEI, 13 rue de Toul, F-59046 Lille, France, 3UFR Pharmacie, EA GRIIOT (4481), Laboratoire de Chimie Analytique, BP 83, F-59006 Lille, France, 4Dipartimento di Chimica, Materiali ed Ingegneria Chimica ‘G. Natta’ Politecnico di Milano, Piazza L. da Vinci 32, I-20133 Milano, Italy, 5CNR-ICRM, Via L. Mancinelli 7, I-20131 Milano, Italy and 6Dipartimento di Scienze Molecolari Agroalimentari, Università di Milano, Via Celoria, 2 I-20133 Milano, Italy
Email: Andrea Mele* - email@example.com
* Corresponding author § Tel.: 39-02-23993006; Fax: 39-02-23993180
Keywords: dynamic cross-polarization; epichlorohydrin; imprinted; insoluble CRYSMEB polymers; solid-state NMR spectroscopy
Beilstein J. Org. Chem. 2015, 11, 2785–2794. doi:10.3762/bjoc.11.299
Received: 22 July 2015 Accepted: 14 December 2015 Published: 30 December 2015
This article is part of the Thematic Series "Superstructures with cyclodextrins: Chemistry and applications III".
Guest Editor: G. Wenz
© 2015 Mallard et al; licensee Beilstein-Institut. License and terms: see end of document.
Abstract The polymerization of partially methylated β-cyclodextrin (CRYSMEB) with epichlorohydrin was carried out in the presence of a known amount of toluene as imprinting agent. Three different preparations (D1, D2 and D3) of imprinted polymers were obtained and characterized by solid-state 13C NMR spectroscopy under cross-polarization magic angle spinning (CP-MAS) conditions. The polymers were prepared by using the same synthetic conditions but with different molar ratios of imprinting agent/monomer, leading to morphologically equivalent materials but with different absorption properties. The main purpose of the work was to find a suitable spectroscopic descriptor accounting for the different imprinting process in three homogeneous polymeric networks. The polymers were characterized by studying the kinetics of the cross-polarization process. This approach is based on variable contact time CP-MAS spectra, referred to as VCP-MAS. The analysis of the VCP-MAS spectra provided two relaxation parameters: TCH (the CP time constant) and T1ρ (the proton spin-lattice relaxation time in the rotating frame). The results and the analysis presented in the paper pointed out that TCH is sensitive to the imprinting process, showing variations related to the toluene/cyclodextrin molar ratio used for the preparation of the materials. Conversely, the observed values of T1ρ did not show dramatic variations with the imprinting protocol, but rather confirmed that the three polymers are morphologically similar. Thus the combined use of TCH and T1ρ can be helpful for the characterization and fine tuning of imprinted polymeric matrices.
http://www.beilstein-journals.org/bjoc/about/openAccess.htm mailto:firstname.lastname@example.org http://dx.doi.org/10.3762%2Fbjoc.11.299
Beilstein J. Org. Chem. 2015, 11, 2785–2794.
Scheme 1: Schematic representation of molecular imprinting technique. i) Polymerization process with toluene-imprinted CRYSMEB and epichloro- hydrin, ii) toluene removal.
Introduction Cyclodextrin polymers are a subject of great interest because of their use in pharmaceutical industry [1,2], analytical chemistry [3-5], wastewater treatment  and food industry [7-9]. Water- insoluble β-cyclodextrin (β-CD) polymers  have been widely described to remove organic pollutants [6,11-13] and heavy metals  from water. The most efficient method for the synthesis of insoluble polymers is to use di- or polyfunc- tional linkers with monomers of cyclodextrins. Different effec- tive crosslinkers have been reported in the literature such as epi- chlorohydrin [15,16], isocyanates [17,18], polycarboxylic acids [19,20] and anhydrides . Following a slightly different ap- proach, Trotta  and his group demonstrated that polymeriza- tion of cyclodextrins with a variety of synthetic equivalents of di- and tetracarboxylic acids provides an easy, efficient and environmentally sustainable route to highly cross-linked, nanoporous polymers commonly referred to as cyclodextrin nanosponges.
One of the most frequently used crosslinker for insoluble poly- mers is epichlorohydrin (EP). In this case, the reaction of β-CD with EP requires very strong alkaline conditions to achieve deprotonation of the hydroxyl groups. Then, EP reacts with the alkoxide to form intra- or inter-ether linkages.
We previously proposed the synthesis  of soluble and insol- uble polymers of a partially secondary rim methylated β-CD (DS = 4.9) commonly called CRYSMEB. In this previous paper, we described the synthesis of imprinted polymers. The imprinting technique is based on interactions between a template and a suitable functional monomer during the prepoly- merization process. Once the template is removed, the resulting product is a cross-linked copolymer matrix with specific recog- nition sites for the template molecule.
As a matter of fact, high-resolution solid-state NMR is a powerful tool to characterize the structure of polymers [23,24] and to study their dynamics [25,26]. Crini has reported previ- ously a solid-state NMR spectroscopy study [27,28] of β-cyclo- dextrin polymers. At this time, no discussion concerning the NMR spectroscopic characterization of insoluble imprinted CRYSMEB polymers has been reported.
The main purpose of these measurements was to explore possible applications of solid-state NMR spectroscopy for the characterization, at the atomic level, of polymers obtained from polydisperse crystalline methyl β-CD (CRYSMEB) and epi- chlorohydrin in the presence of a guest molecule. Particular emphasis is devoted to the determination of possible experi- mental descriptors able to distinguish polymers obtained with the same synthetic route but in the presence of different amounts of imprinting agent, as in the present case. We herein propose an approach based on solid-state 13C NMR techniques such as variable contact time cross-polarization magic angle spinning with dipolar decoupling (VCP-MAS) to describe these new materials. The dynamics of cross-polarization can be conveniently exploited to fingerprint the new materials and to provide information for tailored synthesis.
Results and Discussion The molecular imprinting technique allows the introduction of a molecular memory for drugs [29,30] or volatile organic com- pounds [31,32]. This selective recognition in shape, size and chemical functionality is achieved due to the presence of the target molecule during the polymerization process (Scheme 1).
Initially the target molecules form a complex with the cyclo- dextrin followed by a copolymerization of the imprinted
Beilstein J. Org. Chem. 2015, 11, 2785–2794.
monomers with the crosslinker. The template introduces highly specific sites into the polymeric network and, after removal of the target the polymer is able to rebind the molecule with high selectivity.
Polymers of CRYSMEB were synthesized according to the procedure of Mallard Favier . Our synthetic protocol was chosen to employ a larger ratio of crosslinker to functional monomer to get insoluble polymers. The deprotonation was carried out in aqueous basic media and imprinting was performed in toluene for 20 min before the polymerization process. After the introduction of toluene, a clear solution was systematically observed. The absence of light diffraction, as expected in the case of toluene aggregation, was controlled by recording the UV–vis absorption spectra in the visible region (400–700 nm), outside the absorption range of toluene. As flat- tened signals with absorbances close to zero were obtained for all of the mixtures, one can conclude that toluene was dissolved quantitatively in the aqueous phase. Different molar ratios of toluene/CD were used as reported in Table 1. Toluene was chosen as a template for a paradigmatic representative of aromatic organic compounds. The combination of the two para- meters such as the value of the binding constant between toluene and β-CD (Kf = 158 M−1)  and the high volatility of toluene leads to the conclusion that toluene is a good template for imprinting reactions. According to Ritter , the CD–toluene complex fosters mainly the formation of linear polymers instead of globular polymers and the linear polymer network promotes a more efficient guest binding due to a more effective accessibility of the cavity. These points allow an easy removal of toluene by simple drying in the oven under vacuum. Additionally, the control of the polymer growth leading to linear polymer network provided a sufficiently regular system for the interpretation of the NMR results.
Table 1: Experimental conditions for the synthesis of polymer.a
Polymer EP/CD Toluene/CD
D1 40/1 1/4 D2 40/1 4/1 D3 40/1 3/1
aRatios are molar ratios.
Due to the experimental conditions such as high NaOH concen- tration, high EP/CD ratio and high temperature [15,35], the polymerization process leads exclusively to insoluble cross- linked polymers after EP addition. It should be mentioned that the formation of intralinked bonds between hydroxyl groups and epichlorohydrin was reduced due to the presence of methyl
groups in the outer CD cavity. Under the reaction conditions used (33% NaOH, EP/CD= 40 and T = 6